Rendering Mortars Reinforced with Natural Sheep’s Wool Fibers

The susceptibility of rendering mortars to cracking is a complex phenomenon. Fibers have been incorporated in mortars to ensure the durability of the render and can improve the flexural strength, fracture toughness, and impact resistance of the mortars. Aside from the better cracking performance of fiber reinforced mortars, natural fibers have been a path to reducing the environmental impacts of construction materials. Recycling has high sustainability-related potential as it can both mitigate the amount of waste being inadequately disposed and reduce the consumption of natural raw materials. Studies on the incorporation of waste in civil engineering materials have been growing, and recycled fibers may be feasible to incorporate in mortars. Natural fibers are considered as a viable replacement for synthetic ones. Several studies have investigated vegetal fibers in cementitious composites. However, only a few have focused on the incorporation of waste animal-based fiber. The aim of this work is to analyze the feasibility of the use of natural sheep’s wool fibers on the reinforcement of mortars and in particular to improve their cracking behavior. For this purpose, two different binders were used: cement and cement-lime mortars were produced. The incorporation of 10% and 20% (in volume) of 1.5 cm and 3.0 cm wool fibers was analyzed. The results show that the incorporation of wool fibers increased the ductility of the mortars and improved their mechanical properties.


Introduction
The construction sector has been trying to reduce its environmental impacts. Eco-friendly constituents have been an alternative to develop new cementitious materials. In order to enhance the cracking performance of mortars, the incorporation of natural fibers can contribute to better performance while ensuring a sustainable approach. According to previous studies, natural fibers such as sheep wool may improve the ductility of cementitious composites and also provide an adequate disposal of the waste [1].
The incorporation of fibers enhances a better post-cracking behavior due to the higher fracture toughness, flexural strength, and impact resistance of the mortars [2]. The benefits of fiber reinforcement in cementitious materials depend on the fiber type, their geometry, and their volume ratio and distribution [3]. The use of natural fibers compared to man-made fibers has been achieving environmental, energy, and resource conservation benefits [4]. There are three types of natural fibers: plant-based, mineral-derived, and animal-based. In this paper, the study focused on animal-based fibers, namely sheep's wool fibers.
From the results, it could be seen that the incorporation of wool fibers in rendering mortars with a volumetric ratio of 1:4 (cement: aggregates) and 1:1:6 (cement:air-lime:aggregates) improved the cracking behavior of the materials as the modified mortars, in general, presented a higher flexural strength and a lower modulus of elasticity when compared to the plain mortars.

Experimental Program
The aim of this research was to evaluate the influence of natural fiber waste, namely sheep wool, incorporated in rendering mortars.
Cement mortars and cement-air lime-based mortars were produced. The volumetric proportions were 1:4 (cement: aggregates) and 1:1:6 (cement:air-lime:aggregates). Aside from the binder, the length and volume ratio were parameters used to formulate the analyzed mortars.
Mortars were identified as follows:

Materials
The materials used were cement, air-lime, sand, and wool fibers. The binder used on the cement mortars was CEM II/B-L 32.5 N, according to EN 197-1 [13]. The calcium hydrated lime powder-air lime-used was class CL80-S, according to EN 459-1 [14]. The natural silica sand was previously washed, calibrated, and sieved for a required size distribution. The wool fibers were washed with neutral detergent, and dried at 40 • C. This procedure was applied to remove the impurities. The fiber length was obtained by manually cutting the waste material. The fibers were added in order to ensure a homogeneous dispersion in each mix composition. The homogeneity of the fibers in the mix was implemented by distributing them in a properly closed receptacle and blowing compressed air over them in order to achieve an adequate dispersion before adding to the mix. Figure 1 presents the wool fibers used in the experimental campaign. The apparent bulk density of the constituents of the mortars produced is presented in Table 1.

Methods
All tests carried out in the experimental program are described in Table 3. cracking behavior of the materials as the modified mortars, in general, presented a higher flexural strength and a lower modulus of elasticity when compared to the plain mortars.

Experimental Program
The aim of this research was to evaluate the influence of natural fiber waste, namely sheep wool, incorporated in rendering mortars.
Cement mortars and cement-air lime-based mortars were produced. The volumetric proportions were 1:4 (cement: aggregates) and 1:1:6 (cement:air-lime:aggregates). Aside from the binder, the length and volume ratio were parameters used to formulate the analyzed mortars.

Materials
The materials used were cement, air-lime, sand, and wool fibers. The binder used on the cement mortars was CEM II/B-L 32.5 N, according to EN 197-1 [13]. The calcium hydrated lime powder-air lime-used was class CL80-S, according to EN 459-1 [14]. The natural silica sand was previously washed, calibrated, and sieved for a required size distribution. The wool fibers were washed with neutral detergent, and dried at 40 °C. This procedure was applied to remove the impurities. The fiber length was obtained by manually cutting the waste material. The fibers were added in order to ensure a homogeneous dispersion in each mix composition. The homogeneity of the fibers in the mix was implemented by distributing them in a properly closed receptacle and blowing compressed air over them in order to achieve an adequate dispersion before adding to the mix. Figure 1 presents the wool fibers used in the experimental campaign. The apparent bulk density of the constituents of the mortars produced is presented in Table 1. Table 2 presents the composition of the mortars produced in this work.

Methods
All tests carried out in the experimental program are described in Table 3.
(a) (b)    Table 2 presents the composition of the mortars produced in this work. For the hardened mortar tests, prismatic samples (40 mm × 40 mm × 160 mm) were used, in accordance with European Standards.
For ultra-sound pulse velocity, the direct and indirect methods were used for the measurements. In the direct transmission method, the electrodes are placed on the opposite surfaces of the specimen. In the indirect method, the electrodes are positioned on the same surface of the prism: the transmitter electrode is fixed at a specific point and the receptor moves over the specimen, and at different distances, the transmission time is measured allowing for the velocity to be calculated.
In order to analyze the susceptibility to cracking of the mortars produced in this work, some parameters were calculated. The Center Scientifique et Technique du Bâtiment (CSTB) [15] refers to the dynamic modulus of elasticity and flexural strength ratio (E/σ f ) as indicators of the mortar's ability to resist cracking. This criterion is based on the fact that a lower dynamic modulus of elasticity provides a higher deformation capacity of the material, and a greater flexural strength induces the material to withstand tensions without cracking. Therefore, the tendency to crack due to restrained shrinkage is greater when the ratio between the modulus of elasticity and tensile strength is high.
Another parameter to evaluate the susceptibility to crack is based on the flexural and compressive strengths. The ductility of the material can be associated to this ratio (σ f /σ c ) (i.e., the mortar is considered more ductile when this value is closer to 1). Ductility is a measure of the deformability of the material before fracture. Cracking resistance is correlated with the deformation capacity of the mortar and its ability to absorb stress without cracking [23].
The ability to absorb energy before fracture is correlated with the toughness of the mortar. The fracture toughness was calculated by the total area under the strain-stress curve of the results of flexural strength at 28 days.
Regardless of the binder used, all hardened mortars were cured as specified by EN 1015-11 [21]. The specimens were kept in molds for two days at a temperature of 20 ± 2 • C and a relative humidity of 95 ± 5%. After demolding, all specimens were maintained in the same conditions for a total of seven days. After that, the specimens were kept at 20 ± 2 • C and the relative humidity was reduced to 65 ± 5%, until testing.

Fresh State
The mortar's workability was measured by the consistency test. To improve the comparability of the results, the values were limited to 140 ± 5 mm. The mortars presented a stiff consistence, but an application on a brick was carried out to ensure that an adequate workability was achieved, as shown in Figure 2.
In the direct transmission method, the electrodes are placed on the opposite surfaces of the specimen. In the indirect method, the electrodes are positioned on the same surface of the prism: the transmitter electrode is fixed at a specific point and the receptor moves over the specimen, and at different distances, the transmission time is measured allowing for the velocity to be calculated.
In order to analyze the susceptibility to cracking of the mortars produced in this work, some parameters were calculated. The Center Scientifique et Technique du Bâtiment (CSTB) [15] refers to the dynamic modulus of elasticity and flexural strength ratio (E/σf) as indicators of the mortar's ability to resist cracking. This criterion is based on the fact that a lower dynamic modulus of elasticity provides a higher deformation capacity of the material, and a greater flexural strength induces the material to withstand tensions without cracking. Therefore, the tendency to crack due to restrained shrinkage is greater when the ratio between the modulus of elasticity and tensile strength is high.
Another parameter to evaluate the susceptibility to crack is based on the flexural and compressive strengths. The ductility of the material can be associated to this ratio (σf/σc) (i.e. the mortar is considered more ductile when this value is closer to 1). Ductility is a measure of the deformability of the material before fracture. Cracking resistance is correlated with the deformation capacity of the mortar and its ability to absorb stress without cracking [23].
The ability to absorb energy before fracture is correlated with the toughness of the mortar. The fracture toughness was calculated by the total area under the strain-stress curve of the results of flexural strength at 28 days.
Regardless of the binder used, all hardened mortars were cured as specified by EN 1015-11 [21]. The specimens were kept in molds for two days at a temperature of 20 ± 2 °C and a relative humidity of 95 ± 5%. After demolding, all specimens were maintained in the same conditions for a total of seven days. After that, the specimens were kept at 20 ± 2 °C and the relative humidity was reduced to 65 ± 5%, until testing.

Fresh State
The mortar's workability was measured by the consistency test. To improve the comparability of the results, the values were limited to 140 ± 5 mm. The mortars presented a stiff consistence, but an application on a brick was carried out to ensure that an adequate workability was achieved, as shown in Figure 2. It was noticed that the fibers kept the mortar agglutinated. Although the workability was acceptable, the flor value did not increase due to the fibers' agglutinating action. In order to illustrate this behavior, Figure 3 presents the flow table test of the W 1.5_10%c sample. It was noticed that the fibers kept the mortar agglutinated. Although the workability was acceptable, the flor value did not increase due to the fibers' agglutinating action. In order to illustrate this behavior, Figure 3 presents the flow table test of the W 1.5_10%c sample.  Table 4 presents the results of the fresh mortars' properties.   Table 4 presents the results of the fresh mortars' properties. In all cement-lime mortars, the water/binder ratio was higher than that of the cement mortars. The incorporation of 10% of wool fibers increased the amount of water needed to maintain the workability. This could be due to the morphology of the fiber, which is composed of keratin filaments [5]. However, the incorporation of 20% of fibers again decreased the water/binder ratio to values similar to the control mortar. This trend reversion may be due to the fact that the longer fibers have a lower bulk density and thus a lower weight of incorporated fibers is actually used ( Table 2). The modified mortars presented a lower bulk density than that of the reference mortars.

Dry Bulk Density of the Hardened Mortars
The dry bulk density of the hardened mortars was determined at 28, 90, and 180 days and the results are presented in Figure 4. The same trend as for the fresh state was noticed: the incorporation of wool fibers reduced the dry bulk density of the mortars due to the low bulk density of the fibers. Giosué et al. [11] found similar results (i.e., the bulk density of the reinforced mortars had a decrease of about 13% compared to the control mortar at 28 days).

Dynamic Modulus of Elasticity of the Hardened Mortars
The modulus of elasticity measures the ability of the rendering mortars to absorb deformations. The renders should be able to withstand higher internal stresses without cracking. The dynamic modulus of elasticity was determined at 28  In general, the dry bulk density of the cement mortars decreased from 28 to 90 days. Dry bulk density is defined as the ratio between mass and volume. Thus, the variations in weight and volume during time explain the variations in dry bulk density. In a previous study, a similar trend of decrease from 28 to 90 days was found [24], possibly because the mass reduction overlapped the volume reduction.
The opposite effect occurred in the cement-lime mortars, which presented an increase in this property over time. In fact, cement-lime mortars also have shrinkage with the consequent reduction of volume, and possibly have an increase in weight due to a higher carbonation reaction (by comparison with cement-only mortars). Previous works have shown this same trend for air lime mortars [25].

Dynamic Modulus of Elasticity of the Hardened Mortars
The modulus of elasticity measures the ability of the rendering mortars to absorb deformations. The renders should be able to withstand higher internal stresses without cracking. The dynamic modulus of elasticity was determined at 28, 90, and 180 days. The results are presented in Figures 5  and 6.

Dynamic Modulus of Elasticity of the Hardened Mortars
The modulus of elasticity measures the ability of the rendering mortars to absorb deformations. The renders should be able to withstand higher internal stresses without cracking. The dynamic modulus of elasticity was determined at 28, 90, and 180 days. The results are presented in Figures 5  and 6.  In general, the modified mortars presented a lower modulus of elasticity when compared to the reference mortars. For cement mortars, the modulus of elasticity decreased from 28 to 180 days. This could be attributed to the internal micro-cracking of the mortars over time. The opposite trend occurred in cement-lime mortars (i.e. the modulus of elasticity presented a slight increase from 28 to 90 days).
According to Araya-Letelier et al. [26], the incorporation of pig hair in mortars did not lead to a significant reduction in the dynamic modulus of elasticity. The authors explained this effect by the small amount of total fiber volume incorporated (up to 1.5%).

Ultra-Sound Pulse Velocity of the Hardened Mortars
The ultra-sound pulse velocity test was performed at 28, 90, and 180 days. The results are presented in Table 5. The ultra-sound pulse velocity results showed that the incorporation of fibers

Dynamic Modulus of Elasticity of the Hardened Mortars
The modulus of elasticity measures the ability of the rendering mortars to absorb deformations. The renders should be able to withstand higher internal stresses without cracking. The dynamic modulus of elasticity was determined at 28, 90, and 180 days. The results are presented in Figures 5  and 6.  In general, the modified mortars presented a lower modulus of elasticity when compared to the reference mortars. For cement mortars, the modulus of elasticity decreased from 28 to 180 days. This could be attributed to the internal micro-cracking of the mortars over time. The opposite trend occurred in cement-lime mortars (i.e. the modulus of elasticity presented a slight increase from 28 to 90 days).
According to Araya-Letelier et al. [26], the incorporation of pig hair in mortars did not lead to a significant reduction in the dynamic modulus of elasticity. The authors explained this effect by the small amount of total fiber volume incorporated (up to 1.5%).

Ultra-Sound Pulse Velocity of the Hardened Mortars
The ultra-sound pulse velocity test was performed at 28, 90, and 180 days. The results are presented in Table 5. The ultra-sound pulse velocity results showed that the incorporation of fibers  In general, the modified mortars presented a lower modulus of elasticity when compared to the reference mortars. For cement mortars, the modulus of elasticity decreased from 28 to 180 days. This could be attributed to the internal micro-cracking of the mortars over time. The opposite trend occurred in cement-lime mortars (i.e., the modulus of elasticity presented a slight increase from 28 to 90 days).
According to Araya-Letelier et al. [26], the incorporation of pig hair in mortars did not lead to a significant reduction in the dynamic modulus of elasticity. The authors explained this effect by the small amount of total fiber volume incorporated (up to 1.5%).

Ultra-Sound Pulse Velocity of the Hardened Mortars
The ultra-sound pulse velocity test was performed at 28, 90, and 180 days. The results are presented in Table 5. The ultra-sound pulse velocity results showed that the incorporation of fibers reduced the pulse velocity through the mortar, indicating a decrease in the modulus of elasticity (Table 5).
These results followed the same trend as those of the modulus of elasticity test, as expected. The direct method showed a decrease of the pulse velocity in cement mortars, which could be related to some internal cracks due to shrinkage. According to the indirect method, this reduction is not that significant as it measures the velocity in small distances in the prism, which may detect a more distributed crack pattern and consequent decrease of the pulse velocity, as seen by the high R 2 of the velocity trend lines (Figures 7 and 8).   These results followed the same trend as those of the modulus of elasticity test, as expected. The direct method showed a decrease of the pulse velocity in cement mortars, which could be related to some internal cracks due to shrinkage. According to the indirect method, this reduction is not that significant as it measures the velocity in small distances in the prism, which may detect a more distributed crack pattern and consequent decrease of the pulse velocity, as seen by the high R 2 of the velocity trend lines (Figures 7 and 8). Figures 5 and 6 present the results of the ultra-sound pulse velocity test by the indirect method for the reference mortars and W 1.5_10% mortars. For cement-lime mortars, only W 3.0 cm 10% had an increase of 15% in this property when compared to REF 1:1:6. In general, the modified cement-lime mortars presented a slight decrease in flexural strength. W 1.5 cm 10% obtained the lowest flexural strength, 20% less than the reference mortar. Figure 11 presents the mechanical tests carried out on the mortars.             For cement-lime mortars, only W 3.0 cm 10% had an increase of 15% in this property when compared to REF 1:1:6. In general, the modified cement-lime mortars presented a slight decrease in flexural strength. W 1.5 cm 10% obtained the lowest flexural strength, 20% less than the reference mortar. Figure 11 presents the mechanical tests carried out on the mortars.     Fantilli et al. [5] reached similar conclusions to those of the cement mortars. The modified mortars with wool fibers had an 18% higher flexural strength than that of the control mortar. Araya-Letelier et al. [23] studied the incorporation of natural animal fibers such as pig hair in mortars and also reported an increase in flexural strength of the modified mortars. Giosué et al. [11] reported that a hydraulic-lime mortar with wool fibers achieved about a 30% higher flexural strength than that of the conventional mortar. These previous works explained this increase in flexural strength due to a bridging mechanism.

Flexural and Compressive Strength of the Hardened Mortars
In the compressive strength test, a different trend was found regarding the type of the binder used and the length of the fibers. Indeed, it can be seen that the longer fibers led to an increase in the compressive strength when compared to the cement mortar reference. Modified cement mortars with 1.5 cm of wool fiber presented a slight decrease in compressive strength.
The modified cement-lime mortars obtained a slight reduction of compressive strength compared to the control mortar (REF 1:1:6). W 1.5_20% cl obtained the most significant decrease compared to the reference mortar, about 20%.
Giosué et al. [11] found a decrease in the modified lime-based mortars with wool fibers. The authors reported that the use of fibers reduced the compressive strength of mortars. In agreement with this study, Araya-Letelier et al. [26] found a reduction of compressive strength with the incorporation of animal-based fibers in cement mortars. Figure 12 presents a sample of the modified mortar, where the wool fibers do not produce a significant change in the mortar's appearance.
Fantilli et al. [5] reached similar conclusions to those of the cement mortars. The modified mortars with wool fibers had an 18% higher flexural strength than that of the control mortar. Araya-Letelier et al. [23] studied the incorporation of natural animal fibers such as pig hair in mortars and also reported an increase in flexural strength of the modified mortars. Giosué et al. [11] reported that a hydraulic-lime mortar with wool fibers achieved about a 30% higher flexural strength than that of the conventional mortar. These previous works explained this increase in flexural strength due to a bridging mechanism.
In the compressive strength test, a different trend was found regarding the type of the binder used and the length of the fibers. Indeed, it can be seen that the longer fibers led to an increase in the compressive strength when compared to the cement mortar reference. Modified cement mortars with 1.5 cm of wool fiber presented a slight decrease in compressive strength.
The modified cement-lime mortars obtained a slight reduction of compressive strength compared to the control mortar (REF 1:1:6). W 1.5_20% cl obtained the most significant decrease compared to the reference mortar, about 20%.
Giosué et al. [11] found a decrease in the modified lime-based mortars with wool fibers. The authors reported that the use of fibers reduced the compressive strength of mortars. In agreement with this study, Araya-Letelier et al. [26] found a reduction of compressive strength with the incorporation of animal-based fibers in cement mortars. Figure 12 presents a sample of the modified mortar, where the wool fibers do not produce a significant change in the mortar's appearance.

Cracking Behavior
Restrained shrinkage can be induced by the restrictions imposed on deformations of a rendering mortar. Tensile stresses should be dissipated without cracking of the coating. There are several causes that lead the mortar to crack. In order to evaluate the mortar's susceptibility to cracking, some parameters were considered to enhance the analysis of this phenomena as described above, and the results are presented in Table 6.
The values of fracture toughness are presented in Table 6. An increase in the fracture toughness of the modified cement mortars was noticed. The increment was higher when longer fibers were incorporated, regardless of the incorporation ratio. W 3.0_10%c and W 3.0_20%c attained up to 100% higher toughness values when compared with the reference cement mortar (REF 1:4).
The fracture toughness results of the cement-lime mortars did not present significant changes. These results are in accordance with previous studies [5,27]. Fantilli et al. [5] also obtained a higher fracture toughness with the incorporation of wool fibers in cementitious composites. This can be explained by the fibers' bridging mechanism, since the fibers cross the micro-cracks, preventing

Cracking Behavior
Restrained shrinkage can be induced by the restrictions imposed on deformations of a rendering mortar. Tensile stresses should be dissipated without cracking of the coating. There are several causes that lead the mortar to crack. In order to evaluate the mortar's susceptibility to cracking, some parameters were considered to enhance the analysis of this phenomena as described above, and the results are presented in Table 6.
The values of fracture toughness are presented in Table 6. An increase in the fracture toughness of the modified cement mortars was noticed. The increment was higher when longer fibers were incorporated, regardless of the incorporation ratio. W 3.0_10%c and W 3.0_20%c attained up to 100% higher toughness values when compared with the reference cement mortar (REF 1:4).
The fracture toughness results of the cement-lime mortars did not present significant changes. These results are in accordance with previous studies [5,27]. Fantilli et al. [5] also obtained a higher fracture toughness with the incorporation of wool fibers in cementitious composites. This can be explained by the fibers' bridging mechanism, since the fibers cross the micro-cracks, preventing their propagation and delaying the occurrence of the first crack. Reinforced mortars may withstand tensile load after cracking and exhibit ductile behavior [1,28]. Araya-Letelier et al. [26] found that the incorporation of animal-based fibers, namely pig hair, increased the fracture toughness of the fiber-reinforced mortars. The authors related this increment to the increase in the impact energy absorption capacity of the mortars due to the addition of fibers. In this work, it was reported that the post-cracking behavior of the modified mortars was improved by up to 55% higher energy absorbed at failure.
Considering these factors, all the modified mortars evaluated in this work were less susceptible to cracking. However, the cement-lime mortars presented more ductility than the cement mortars. The incorporation of 20% of 1.5 cm long wool fibers in cement-lime mortars presented the best results regarding ductility. Table 6 presents the results of tests on the hardened mortars.

Open Porosity
The open porosity test determines the volume of interconnected voids in the mortars, in percentage. This property is correlated with the ultra-sound pulse velocity and modulus of elasticity as well as the mechanical strength and water tightness behavior. Table 7 presents the results of the open porosity test. The results of the open porosity test confirmed the expectations. In general, the incorporation of fibers increased the volume of pores of the modified mortars. W 3.0_20%c was an exception, as it presented a reduction of 1.5% of total open porosity compared to the control cement mortar. The incorporation of 10% of wool fibers in cement mortars presented the same values, regardless of the length of the fibers.
The cement-lime modified mortars exhibited a greater increase in the volume of pores than that of the cement mortars. W 3.0_20% cl obtained an increase of about 6.5% of total open porosity compared to REF 1:1:6.
Giosué et al. [11] also noticed an increase (32%) of total open porosity in hydraulic lime-mortars with the incorporation of 25% of wool fibers when compared to the control mortar. The increase in open porosity of the modified mortars could be explained by the fiber-matrix interfacial bond that is thought to be less efficient than that of the sand-matrix.

Conclusions
From the results of the experimental campaign, it was concluded that the incorporation of wool fibers in rendering mortars presented a satisfactory performance concerning the mechanical and cracking behavior. All of the modified mortars presented less susceptibility to cracking when compared with the mortars without fibers, based on the parameters evaluated.
In general, the reinforced mortars presented a decrease in the dynamic modulus of elasticity, which can be considered an advantage of the incorporation of wool fibers. W 3.0_10%c and W 1.5_10%cl obtained a similar decrease of 20% of modulus of elasticity when compared to the control mortar.
Regarding flexural strength, the modified cement mortars presented an increase when compared to the reference mortar. The addition of longer fibers enhanced the mechanical strength of the mortars. W 3.0_20%c obtained an increase of 40% in flexural strength when compared to REF 1:4. The cement-lime modified mortars obtained a slight reduction in flexural strength, with the exception of W 3.0_10%cl.
The dynamic modulus of elasticity and flexural strength ratio (E/σ f ) was analyzed as an indicator of the mortars' ability to resist cracking. It could be seen that all of the modified mortars, regardless of the binder used, presented a lower (E/σ f ) ratio, which could lead to a lesser tendency to crack due to restrained shrinkage when compared to the reference mortars.
The ratio (σ f /σ c ) is related to the mortar's ductility. According to the results, all the modified mortars presented a higher ratio (σ f /σ c ) compared to the reference mortars, which allows concluding that the incorporation of fibers increased the ductility of those mortars, based on this parameter.
Regarding fracture toughness, the modified cement mortars presented improvements. In fact, the toughness increment was higher when longer fibers were incorporated. However, for the cement-lime mortars, the toughness results did not present any significant contribution of the incorporation of the fibers.
Besides the analyzed parameters related with the cracking behavior, it was also found that, concerning compressive strength, the incorporation of longer fibers in cement mortars (W 3.0_10%c and W 3.0_20%c) resulted in an increase.
The results obtained in this work identify the advantages of the addition of the natural wool fibers in rendering mortars, namely concerning the improvement in the mechanical, and in particular of the cracking behavior.